NANO EXPRESS

Open Access

Conductance of Graphene Nanoribbon Junctions and the Tight Binding Model Y Wu, PA Childs*

Abstract Planar carbon-based electronic devices, including metal/semiconductor junctions, transistors and interconnects, can now be formed from patterned sheets of graphene. Most simulations of charge transport within graphene-based electronic devices assume an energy band structure based on a nearest-neighbour tight binding analysis. In this paper, the energy band structure and conductance of graphene nanoribbons and metal/semiconductor junctions are obtained using a third nearest-neighbour tight binding analysis in conjunction with an efficient nonequilibrium Green’s function formalism. We find significant differences in both the energy band structure and conductance obtained with the two approximations. Introduction Since the report of the preparation of graphene by Novoselov et al. [1] in 2004, there has been an enormous and rapid growth in interest in the material. Of all the allotropes of carbon, graphene is of particular interest to the semiconductor industry as it is compatible with planar technology. Although graphene is metallic, it can be tailored to form semiconducting nanoribbons, junctions and circuits by lithographic techniques. Simulations of charge transport within devices based on this new technology exploit established techniques for low dimensional structures [2,3]. The current flowing through a semiconducting nanoribbon formed between two metallic contacts has been established using a nonequilibrium Green’s Function (NEGF) formalism based coupled with an energy band structure derived using a tight binding Hamiltonian [4-7]. To minimise computation time, the nearest-neighbour tight binding approximation is commonly used to determine the energy states and overlap is ignored. This assumption has also been used for calculating the energy states of other carbon-based materials such as carbon nanotubes [8] and carbon nanocones [9]. Recently, Reich et al. [10] have demonstrated that this approximation is only valid close to the K points, and a tight binding approach including up to third nearestneighbours gives a better approximation to the energy dispersion over the entire Brillouin zone. * Correspondence: [email protected] School of Electronic, Electrical and Computer Engineering, University of Birmingham, B15 2TT, Birmingham, UK.

In this paper, we simulate charge transport in a graphene nanoribbon and a nanoribbon junction using a NEGF based on a third nearest-neighbour tight binding energy dispersion. For transport studies in nanoribbons and junctions, the formulation of the problem differs from that required for bulk graphene. Third nearestneighbour interactions introduce additional exchange and overlap integrals significantly modifying the Green’s function. Calculation of device characteristics is facilitated by the inclusion of a Sancho-Rubio [11] iterative scheme, modified by the inclusion of third nearestneighbour interactions, for the calculation of the selfenergies. We find that the conductance is significantly altered compared with that obtained based on the nearest-neighbour tight binding dispersion even in an isolated nanoribbon. Hong et al. [12] observed that the conductance is modified (increased as well as decreased) by the presence of defects within the lattice. Our results show that details of the band structure can significantly modify the observed conductivities when defects are included in the structure.

Theory The basis for our analysis is the hexagonal graphene lattice shown in Figure 1. a1 and b1 are the principal vectors of the unit cell containing two carbon atoms belonging to the two sub-lattices. Atoms on the concentric circles of increasing radius correspond to the nearest-neighbours, second nearest-neighbours and third nearest-neighbours, respectively.

© 2010 Wu and Childs. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Wu and Childs Nanoscale Res Lett 2011, 6:62 http://www.nanoscalereslett.com/content/6/1/62

Page 2 of 5

For the nth row of the above equation, we have H n,n −1 n −1 + H n,n n + H n,n +1 n +1

(3)

− E(S n,n −1 n −1 + S n,n n + S n,n +1 n +1) = 0

Considering the energy dispersion in the direction of charge transport, the Bloch form of the wavefunction ensures that n~eikn. Substitution of n into the above equation yields the secular equation det[H n,n −1e −ik + H n,n + H n,n +1e ik

(4)

− E(S n,n −1e −ik + S n,n + S n,n +1e ik )] = 0

Figure 1 Armchair-edge graphene metal (index N = 23)/ semiconductor (index N = 13) junction. The rectangle shows the semiconductor unit cell, and the concentric circles of increasing radius show first, second and third nearest-neighbours, respectively.

Saito et al. [8] derived the dispersion relation below using a nearest-neighbour tight binding analysis including the overlap integral s0. E ± (k ) =

2 p 0 f (k )

(1)

1 s 0 f (k )

Here, f(k) = 3 + 2 cos k · a1 +2 cos k · b1 + 2 cos k · (a1 - b1) and the parameters, ε2p, g0 and s0 are obtained by fitting to experimental results or ab initio calculations. Most analyses of charge transport in graphene-based structures simplify the result further by ignoring s0. Reich et al. [10] derived the dispersion relation for graphene based on third nearest-neighbours. In this work, the energy band structure of a graphene nanoribbon including third nearest-neighbour interactions is obtained from the block Hamiltonian and overlap matrices given below for the unit cell defined by the rectangle in Figure 1. ⎤ ⎡ 0 ⎤ ⎡ S 0,0 S 0,1 ⎥⎢ ⎢ ⎥ ⎥⎢ ⎥ ⎢ ⎥ ⎢ n ⎥ S n,n −1 S n,n S n,n +1 E⎢ ⎥⎢ ⎢ ⎥ ⎥⎢ ⎥ ⎢ ⎢ S N ,N −1 S N ,N ⎥⎦ ⎢⎣ N ⎥⎦ ⎣ ⎤ ⎡ 0 ⎡ H 0,0 H 0,1 ⎥⎢ ⎢ ⎥⎢ ⎢ ⎥ ⎢ n H n,n −1 H n,n H n,n +1 =⎢ ⎥⎢ ⎢ ⎥⎢ ⎢ ⎢ H N ,N −1 H N ,N ⎥⎦ ⎢⎣ N ⎣

In the case of first nearest approximation without orbital overlap, Sn,n-1 and Sn,n+1 are empty matrices. To facilitate comparison with published results, we use an armchair-edge with index [13] N = 13 as our model nanoribbon. In the paper by Reich, tight binding parameters were obtained by fitting the band structure to that obtained by ab initio calculations. Recently, Kundo [14] has reported a set of tight biding parameters based on fitting to a first principle calculation but more directly related to the physical quantities of interest. These parameters have been utilised in our calculation and are presented below for third nearest-neighbour interactions (Table 1). Figure 2 compares the energy band structure of the modelled armchair-edge graphene nanoribbon obtained from the first nearest-neighbour tight binding method with that obtained by including up to third nearestneighbours. Agreement is reasonable close to the K point but significant discrepancies occur at higher energies.

Conductance of Graphene Nanoribbons and Junctions Conductance in graphene nanoribbons and metal/semiconductor junctions is determined using an efficient nonequilibrium Green’s function formalism described by Li and Lu [15]. The retarded Green’s function is given by G = [E + S − H − Σ L − Σ R ] −1

⎤ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎦

(2)

(5)

Here, E + = E + ih and h is a small positive energy value (10-5 eV in this simulation) which circumvents the singular point of the matrix inversion [16]. H is a tight binding Hamiltonian matrix including up to third nearest-neighbours, and S is the overlap matrix. Open Table 1 Tight binding parameters [14] Neighbours

E2p(eV)

g0(eV)

g1(eV)

g2(eV)

s0

s1

s2

3rd-nearest

-0.45

-2.78

-0.15

-0.095

0.117

0.004

0.002

Wu and Childs Nanoscale Res Lett 2011, 6:62 http://www.nanoscalereslett.com/content/6/1/62

(b)

2

2

1.5

1.5

1

1

Energy E (eV)

Energy E (eV)

(a)

Page 3 of 5

0.5 0 -0.5

0.5 0 -0.5

-1

-1

-1.5

-1.5

-2 -3

-2

-1

0

1

2

3

-2 -3

-2

-1

0

1

2

3

Ka

Ka

Figure 2 Energy band structure of an N = 13 armchair graphene nanoribbon, a obtained from the first nearest-neighbour tight binding method and b including third nearest-neighbours.

boundary conditions are included through the left and right self-energy matrix elements, ΣL.R. The self-energies are independently evaluated through an iterative scheme described by Sancho et al. [11], modified to include third nearest-neighbour interactions. Determination of the retarded Green’s function through equation 5 is facilitated by the inclusion of the body of the device in the right-hand contact through the recursive scheme described in ref. [15]. We will now outline the numerical procedure for deriving the conductance with third nearest-neighbour interactions included. Figure 3 shows a schematic of the unit cell labelling used to formulate the Green’s function. We calculate the surface retarded Green’s functions of the left and right leads by g 0L,0

+

= [E S 0,0 − H 0,0

− (E S 0,−1 − H 0,−1) ] −1 +

(6)

where ti and ti are defined by −1 2 t i = (I − t i −1 t i −1 − t i −1t i −1) t i −1

(10)

−1 2 ti = (I − t i −1 t i −1 − t i −1t i −1) t i −1

(11)

and t 0 = (E + S 0,0 − H 0,0 ) −1(E + S 0,−1 − H 0,−1)

(12)

t0 = (E + S 0,0 − H 0,0 ) −1(E + S −1,0 − H −1,0 )

(13)

The process is repeated until t 0 t0 < with δ arbitrarily small. The nonzero elements of the self-energies Σ1L,1 and Σ RM, M can be then obtained by

R gM +1, M+1

+

+

= [E S 0,0 − H 0,0 − (E S −1,0 − H −1,0 ) ]

−1

(7)

where θ and are the appropriate transfer matrices calculated from the following iterative procedure.

= t 0 + t0t 1 + t0 t1 t 2 + + t0 t1 t2 t n

(8)

= t0 + t 0 t1 + t 0t 1 t2 + + t 0t 1t 2 tn

(9)

Σ1L,1 = (E + S1,0 − H1,0 )g 0R,0(E + S 0,1 − H 0,1)

(14)

R + Σ RM, M = (E + S 0,1 − H 0,1)g M +1, M+1( E S1,0 − H 1,0 )

(15)

The conductance is obtained from the relation G(E) =

2e 2 T (E) h

(16)

where the transmission coefficient is obtained from T ( E ) = Tr[Γ LGΓ RG †],

Figure 3 Schematic showing the unit cell labelling used to formulate the Green’s function.

(17)

with ΓL,R = i[ΣL,R - (ΣL,R)†]. Figure 4a, b compares the conductance of a graphene armchair-edge nanoribbon of index N = 13 and metal/ semiconductor junction formed with the nanoribbon

Wu and Childs Nanoscale Res Lett 2011, 6:62 http://www.nanoscalereslett.com/content/6/1/62

Conductance 2e /h

2

(b)

2

(a) 4 Conductance 2e /h

Page 4 of 5

3 2 1 0

-1

0

1

E (eV)

4 3 2 1 0

-1

0

1

E (eV)

Figure 4 Conductance vs Energy for the junction shown in Figure 1, a using first nearest-neighbour parameters and b using third nearest-neighbours parameters. Dotted lines are for N = 13 armchair nanoribbon, solid lines are for ideal metal/semiconductor junctions, dot– dash lines and dash lines are for junctions with a single defect type A (triangle in Figure 1) and type B (rectangle in Figure 1) respectively.

assuming first and third nearest-neighbour interactions, respectively. For graphene nanoribbons, differences are observed in the step-like structure, reflecting differences in the calculated band structure. When only first nearest-neighbour interactions are considered, the conductance of the conduction and valence bands is always symmetrical as determined by the formulation of the energy dispersion relation, equation 1. In the case of graphene nanoribbons, the conductance within a few electron volts of the Fermi energy is symmetrical for both first and third nearest-neighbour interactions. However, it is notable that at higher energies, overlap integrals introduced by third nearest-neighbour interactions result in asymmetry between the conductance in the conduction and valence bands. For metal/semiconductor junctions, significant differences in conductivity occur even at low energies due to mismatches of the sub-bands. Asymmetry in the conduction and valence band conductance (absent for first nearest-neighbour interactions) is also apparent when third nearestneighbour interactions are included in the Green’s function. Differences are also seen when defects are incorporated within a metal/semiconductor junction, an interesting system explored by Hong et.al. [12]. In this work, vacancies are introduced in the lattice at the positions marked by the solid rectangle and triangle in Figure 1 and the conductance obtained in each case. Hong et al. derive a coupling term associated with differences in band structure. For third nearest-neighbour, the solution to the coupling strength must be derived numerically.

Conclusions In this paper, we have determined the energy band structure of graphene nanoribbons and conductance of nanoribbons and graphene metal/semiconductor

junctions using a NEGF formalism based on the tight binding method approximated to first nearest-neighbour and third nearest-neighbour. Significant differences are observed, suggesting the commonly used first nearestneighbour approximation may not be sufficiently accurate in some circumstances. The most notable differences are observed when defects are introduced in the metal/semiconductor junctions. Received: 9 July 2010 Accepted: 9 September 2010 Published: 7 October 2010 References 1. Novoselov KS, et al: Two-dimensional gas of massless Dirac fermions in graphene. Nature 2005, 438:197-200. 2. Cresti A, et al: Charge transport in disordered graphene-based low dimensional materials. Nano Res 2008, 1:361-394. 3. Neto A, et al: The electronic properties of graphene. Rev Mod Phys 2009, 81:109-162. 4. Golizadeh-Mojarad R, et al: Atomistic non-equilibrium Green’s function simulations of Graphene nano-ribbons in the quantum hall regime. J Comput Electron 2008, 7:407-410. 5. Liang G, et al: Ballistic graphene nanoribbon metal-oxide-semiconductor field-effect transistors: a full real-space quantum transport simulation. J Appl Phys 2007, 102:054307. 6. Zhao P, Guo J: Modeling edge effects in graphene nanoribbon fieldeffect transistors with real and mode space methods. J Appl Phys 2009, 105:4503. 7. Odili D, et al: Modeling charge transport in graphene nanoribbons and carbon nanotubes using a Schrödinger-Poisson solver. J Appl Phys 2009, 106:024509. 8. Saito R, et al: Physical Properties of Carbon Nanotubes. Imperial College Press, London; 1998. 9. Chen J, et al: Low-energy electronic states of carbon nanocones in an electric field. Nano Micro Lett 2010, 2:121-125. 10. Reich S, et al: Tight-binding description of graphene. Phys Rev B 2002, 66:035412. 11. Sancho M, et al: Quick iterative scheme for the calculation of transfer matrices: application to Mo (100). J Phys F: Metal Phys 1984, 14:1205-1215. 12. Hong S, et al: Metal-semiconductor junction of graphene nanoribbons. Appl Phys Lett 2008, 92:083107. 13. Nakada K, et al: Edge state in graphene ribbons: nanometer size effect and edge shape dependence. Phys Rev B 1996, 54:17954-17961.

Wu and Childs Nanoscale Res Lett 2011, 6:62 http://www.nanoscalereslett.com/content/6/1/62

Page 5 of 5

14. Kundu R: Tight binding parameters for graphene. 2009, Arxiv preprint arXiv:0907.4264. 15. Li TC, Lu S-P: Quantum conductance of graphene nanoribbons with edge defects. Phys Rev B 2008, 77:085408. 16. Datta S: Quantum Transport: Atom to Transistor Cambridge University Press, Cambridge; 2005. doi:10.1007/s11671-010-9791-y Cite this article as: Wu and Childs: Conductance of Graphene Nanoribbon Junctions and the Tight Binding Model. Nanoscale Res Lett 2011 6:62.

Submit your manuscript to a journal and benefit from: 7 Convenient online submission 7 Rigorous peer review 7 Immediate publication on acceptance 7 Open access: articles freely available online 7 High visibility within the field 7 Retaining the copyright to your article

Submit your next manuscript at 7 springeropen.com